Name of Department (Times New Roman 12pt/Bold)Concrete Circular Columns
A confinement model for FRP confined normal- and high-strength concrete circular columns
is established in this study. In addition to the column parameters used in existing models, a
new parameter is added for estimating the compressive strength of FRP confined concrete.
The proposed model is able to predict the ultimate condition of FRP confined concrete
columns that have similar unconfined concrete strength and confining pressure but significant
differences in the jacket stiffness. The proposed model was then verified using a database of
574 FRP confined concrete circular columns with different types of FRP. This database
covers unconfined concrete strength between 15 MPa and 170 MPa and specimens with a
diameter ranging from 51 mm to 406 mm. Furthermore, this database includes specimens
with a variety of FRP types: carbon FRP (CFRP), glass FRP (GFRP), high-modulus carbon
FRP, aramid FRP (AFRP), CFRP tube, ultra-high-modulus CFRP tube, and AFRP tube.
Finally, verifying the proposed model with the extensive database revealed that the proposed
model has a very good level of prediction of the experimental results.
CE Database subject headings: Fiber reinforced polymer; Confinement; Concrete columns;
Compressive strength; Strain; High-strength concrete.
1 Ph.D. Candidate, School of Civil, Mining and Environmental Engineering, University of Wollongong,
Wollongong, NSW 2522, Australia; Formerly, Lecturer, Faculty of Civil Engineering, HCMC University of
Technology, Ho Chi Minh City 70000, Vietnam. Email: [email protected]
2 Associate Professor, School of Civil, Mining and Environmental Engineering, University of Wollongong, NSW
2522, Australia (corresponding author). Email: [email protected]
Fiber-reinforced polymer (FRP) has been commonly used in practice as a confining material
for concrete columns to enhance significantly their strength and ductility. The use of FRP has
been applied to both normal strength concrete (NSC) and high strength concrete (HSC) under
both concentric and eccentric loads (Mirmiran et al. 1998; Hadi and Li 2004; Hadi 2006; Hadi
and Widiarsa 2012; Hadi et al. 2013; Pham et al. 2013). This use of FRP in industry has
required design guidelines for these applications. Many confinement models for FRP confined
concrete columns were therefore proposed to simulate the behavior of confined concrete
columns (Karbhari and Gao 1997; Karabinis and Rousakis 2002; Lam and Teng 2003; Berthet
et al. 2006; Matthys et al. 2006; Jiang and Teng 2007; Wu and Zhou 2010; Yazici and Hadi
2012). Most of the existing models are applicable for FRP confined NSC columns with
exceptions of the models by Mandal et al. (2005), Cui and Sheikh (2010a), Berthet et al.
(2006), and Xiao et al. (2010). It is noted that the model by Xiao et al. (2010) was developed
for actively confined HSC. Therefore, it is necessary to develop a model to cover a wide
range of unconfined concrete strength from NSC to HSC.
This study presents an overview of the existing models for FRP confined concrete circular
sections. Column parameters affecting the ultimate condition of FRP confined concrete are
discussed. In addition to the column parameters used in existing models, the proposed model
for estimating the compressive strength of FRP confined concrete includes a new column
parameter. The proposed strength model was established based on the principles of artificial
neural networks (ANN) while the proposed strain model was developed using the energy
approach. This study also collated an extensive database with varied FRP types to calibrate
and verify the proposed model.
Mechanism of confinement
In this section, the key assumptions of existing strength models are studied and discussed.
Most models for calculating the compressive strength of confined concrete have the following
’ are the compressive strength of confined concrete and unconfined concrete,
respectively, fl is the lateral confining pressure, and k1 is the confinement effectiveness
coefficient. The above form which was initially proposed by Richart et al. (1928) is based on
tests of actively confined concrete with a value of 4.1 for k1. The confining pressure could be
calculated as follows:
where ff is the tensile strength of FRP determined from flat coupon tests, t is the thickness of
FRP, and d is the section diameter.
In addition, a few of the existing models had proposed a modified format of the above
equation in the following form:
where n is calibrated from a database.
In general, the value of k1 could be a constant or a function of confinement ratio (fl/ fco ’ ). This
coefficient was attained by calibrating a database (Khalili and Fardis 1982; Karbhari and Gao
1997; Samaan et al. 1998; Toutanji 1999; Xiao and Wu 2000; Lam and Teng 2003; Bisby et
al. 2005; Berthet et al. 2006; Matthys et al. 2006; Youssef et al. 2007). So, the accuracy of
this coefficient depends on the size and reliability of the database used in their calibration.
Ozbakkaloglu et al. (2013) have conducted an overview of 88 confinement models for FRP
confined concrete in circular sections. From that study, it can be seen that the majority of
equations for calculating the compressive strength of confined concrete are a function of the
unconfined concrete strength (fco ’ ) and the confining pressure (fl).
A few other studies presented their models based on different forms or approaches. Mander et
al. (1988) proposed a different form developed from a multiaxial failure surface for estimating
the compressive strength of confined concrete as follows:
f. ..ff 2
947 125422541 (4)
The Mohr-Columb failure criterion was adopted by Shehata et al. (2002) and Li et al. (2003)
to propose the following equation:
where is the angle of internal friction of concrete.
Wu and Zhou (2010) adopted Hoek-Brown failure criterion (Hoek and Brown 1980) to
propose the following equation for strength estimation:
As mentioned above, there are a few approaches to develop an equation for strength
estimation of confined concrete. All of the above models assumed that the compressive
strength of confined concrete is a function of the unconfined compressive strength of concrete
and the confining pressure. In the following sections, this study will show some specimens
which have been reported in the database and conducted by different researchers. They had
very similar values of unconfined concrete strength and confining pressure but they had
significant differences in the compressive strength of the confined concrete.
The test database used in this study contains experimental results of 574 FRP confined
circular plain concrete columns. The test database was collated from several experimental
tests being conducted over the past few decades (Ahmad et al. 1991; Nanni and Bradford
1995; Karbhari and Gao 1997; Mirmiran et al. 1998; o h tt n ossi r ; Xiao and
Wu 2000; Zhang et al. 2000; Lin and Chen 2001; Karabinis and Rousakis 2002; Shehata et al.
2002; Li et al. 2003; Lam and Teng 2004; Lin and Liao 2004; Theriault et al. 2004; Au and
Buyukozturk 2005; Berthet et al. 2005; Mandal et al. 2005; Matthys et al. 2005; Green et al.
2006; Lam et al. 2006; Saenz and Pantelides 2006; Shao et al. 2006; Silva and Rodrigues
2006; Wu et al. 2006; Yan et al. 2006; Almusallam 2007; Jiang and Teng 2007; Teng et al.
2007; Valdmanis et al. 2007; Youssef et al. 2007; Tamuzs et al. 2008; Wang and Wu 2008;
Wong et al. 2008; Wu et al. 2008; Wu et al. 2009; Aire et al. 2010; Benzaid et al. 2010; Cui
and Sheikh 2010b; Lee et al. 2010; Smith et al. 2010; Xiao et al. 2010). Other tests were
conducted by Evans et al. (2008), Howie and Karbhari (1994), Ilki et al. (2002), Issa and
Karam (2004), Miyauchi et al. (1999), Ongpeng (2006), Owen (1998), Rousakis et al. (2003),
Suter and Pinzelli (2001), Comert et al. (2009), Micelli et al. (2001), Rousakis (2001), Chan
et al. (2007), Kashyap (2007), and Wang (2008) as cited in Ozbakkaloglu and Lim (2013).
The database contains a variety of FRP types: carbon FRP (CFRP, 317 specimens), glass FRP
(GFRP, 119 specimens), high-modulus carbon FRP (HM CFRP, 45 specimens), aramid FRP
(AFRP, 35 specimens), CFRP tube (28 specimens), ultra-high-modulus CFRP (UHM CFRP,
7 specimens) tube, and AFRP tube (23 specimens). The unconfined concrete strength in the
database ranges between 15 MPa and 170 MPa. The diameter of specimens varies between 51
mm and 406 mm. The test database covers a wide range of FRP confinement levels (fl/fco ’ ).
The compressive strength of the most heavily confined specimen and the least lightly
confined specimen increased by about 440% and 10%, respectively. All specimens exhibiting
a stress-strain curve with a descending branch, which is defined below, and specimens which
showed a negligible strength increase were excluded from the database. Specimens damaged
by premature rupture of FRP were also excluded from the database.
The stress-strain relationship of FRP confined concrete is classified into two types: an
ascending branch and a descending branch as shown in Fig. 1. This study only concerns the
ascending branch type specimens. There are three key points of the stress-strain curve which
are the ultimate strength of unconfined concrete, the transition point, and the ultimate strength
of the confined concrete. The stress-strain relationship proposed by Lam and Teng (2003) is
widely accepted and was adopted by ACI 440.2R (2008). This stress-strain relationship was
adopted herein for FRP confined circular plain concrete specimens. It is also commonly
accepted that the stress-strain relation is bi-linear. As such, once the ultimate stress/strain is
precisely determined, the stress-strain curves should not be much different even though they
could be calculated by different models. Therefore, determining the ultimate condition of FRP
confined concrete plays an important role in a confinement model.
Effect of confinement stiffness
As mentioned above, many of the existing models have confirmed that only the unconfined
concrete strength and the confining pressure affect significantly the compressive strength of
FRP confined concrete. However, Teng et al. (2009) indicated that there were specimens with
very similar unconfined concrete strength and confining pressure but they yielded different
compressive strength of confined concrete. Teng et al. (2009) then introduced two new
parameters that affect the compressive strength of confined concrete. The two new parameters
are the confinement stiffness ratio (k) and the strain ratio ():
where Ef is the plastic modulus of FRP, co is the axial strain at peak stress of unconfined
concrete, and fe is the actual rupture strain of FRP in the hoop direction. The compressive
strength of confined concrete was calculated as:
cc 010531 (9)
The equation above is used for specimens having k greater than 0.01. Table 1 was extracted
from the full database to show that even though some specimens had very similar unconfined
concrete strength and confining pressure, they had significant differences in the confined
compressive strength. Due to space limitation, only six groups of typical test results are
presented in Table 1. It is noted that the specimens in each group of Table 1 were conducted
by different researchers and are named “pseudo-identical specimens”. These specimens had
different confinement stiffness ratio and strain ratio. As a result, their strengths were different
as based on Teng et al.’s model (2009).
Interestingly, Eq. 9 shows that the compressive strength of confined concrete must be in direct
proportion to the value of (k - 0.01) It is found in Group 2 of Table 1 that the Columns 2a
had the value of (k - 0.01)being greater than that of Columns 2b but the value of fcc ’ of
Columns 2a is much smaller than that of Columns 2b. Similarly, the columns in Groups 3 and
6 also have the same indication. This observation may indicate that using the two new
parameters do not well predict the compressive strength of confined concrete. In such cases,
the FRP thickness ratio (t/d in Table 1) can reflect the difference in these “pseudo-identical
specimens” that have the same unconfined concrete strength and confining pressure but
different confined compressive strength. The FRP thickness ratio is always in direct
proportion to the compressive strength of confined concrete as confirmed by the database.
Furthermore, Pham and Hadi (2014b) also took the FRP thickness ratio (t/d) into account for
calculating the compressive strength of FRP confined rectangular columns. Therefore, this
study takes into account the unconfined concrete strength, the confining pressure and the FRP
thickness ratio to calculate the compressive strength of confined concrete.
Strength model for FRP confined circular concrete columns
The proposed strength model
In order to calculate the compressive strength of FRP confined concrete columns, this study
adopted a method proposed by Pham and Hadi (2014a) to generate a simple-form equation
from a trained ANN. Pham and Hadi (2014a) concluded that the output could be calculated by
multiplying the inputs by a proportional matrix if the proposed ANN is trained and yields
good results. The inputs herein are column parameters of FRP confined concrete while the
output is its confined compressive strength. It means that the compressive strength of
confined concrete could be predicted by multiplying the column parameters by the
proportional matrix. The proportional matrix is obtained by multiplying the input weight
matrix by the layer weight matrix and normalizing the inputs and the outputs. Details of this
method and definitions of some concepts could be found in the study by Pham and Hadi
As mentioned above, the ratio between the FRP thickness and the section diameter affects the
compressive strength of FRP confined concrete. Thus, three column parameters are
considered in this model, which are the unconfined concrete strength fco ’ (MPa), the confining
pressure fl (MPa), and the ratio between the FRP thickness and the section diameter t/d (%).
The compressive strength of FRP confined circular columns could be calculated as follows:
where the confining pressure fl is estimated from Eq. 2.
The proposed model could be used to estimate the compressive strength of confined concrete
made of a variety of FRP types including CFRP, GFRP, AFRP, HM CFRP, UHM CFRP tube,
CFRP tube, and AFRP tube. In addition, it is noted that Eq. 10 covers columns that have
parameters in the ranges shown in Table 2.
Verification of the strength model
The proposed strength model was verified by the database including seven types of FRP and a
wide range of compressive strength of unconfined concrete. Fig. 2 shows 574 data points of
the predicted compressive strength of FRP confined concrete versus their experimental
results. As shown in Fig. 2, the proposed strength model could predict the compressive
strength of FRP-confined normal- and high-strength concrete circular columns. The
compressive strength of unconfined concrete ranges between 15 MPa and 170 MPa. In
addition, the normalized predicted compressive strengths of confined columns versus their
normalized experimental results are shown in Fig. 3. Five existing models were studied in this
verification (Berthet et al. 2006; Matthys et al. 2006; Teng et al. 2009; Wu and Wang 2009;
Yazici and Hadi 2012). The average absolute error (AAE), which is calculated using Eq. 11,
of the above models ranges between 11.54% and 15.97%. The proposed model shows the
smallest value of AAE (9.88%) among these models.
where pre is the model predictions, exp is the experimental results, and N is the total number
of specimens. The mean square error (MSE) and the standard deviation (SD) are also
calculated to assess the accuracy of the models:
Furthermore, the equation of the best-fit line (in the format y=ax) and the correlation factor
(R 2 ) in each model are reported. The five models above have a correlation factor ranging from
0.76 to 0.79 whil th t f tor of th propos mo ls is .88. Th v lu of “a” of th qu tion
of the best-fit line could depict that the model is conservative (a < 1) or vice versa (a > 1). As
can be easily seen in Fig. 3 that the models by Berthet et al. (2006), Teng et al. (2009), Wu
and Wang (2009), and Yazici and Hadi (2012) are conservative while the model by Matthys
et al. (2006) is less-conservative. Interestingly, the value of “a” of the proposed strength
model is equal to 1. In addition, the error of the strength models was statistically verified and
presented in Fig. 4.
Discussion of the proposed strength model
Figs. 3-4 show that Eq. 10 compares well with the experimental data. However, the constant
(value of 13) at the end of the equation may cause a considerable error in estimating the
compressive strength of a specimen having low unconfined concrete strength and confining
pressure. Consequently, the following equation is proposed as an approximation:
To verify the performance of Eq. 14, Fig. 5 shows the prediction results versus the
experimental results. The error calculated from the prediction of Eq. 14 is slightly higher as
compared to that of Eq. 10.
Strain model for FRP confined circular concrete columns
Strain energy absorption
The proposed strain model was developed based on the energy approach that was proposed by
Pham and Hadi (2013). Pham and Hadi (2013) concluded that there is a linear relationship
between the additional volumetric strain energy absorbed by a column core (Ucc) and the
volumetric strain energy absorbed by FRP (Uf). When the strain of confined concrete is below
the peak strain of the corresponding unconfined concrete, the effect of FRP is negligible.
Thus, it is assumed that the additional energy in the column core equals the area under the
experimental stress–strain curves starting from the value of unconfined concrete strain. The
additional volumetric strain energy absorbed by a column core (Ucc) is calculated as follows:
where fc is the axial stress of the concrete, dc is an increment of the axial strain, Ucc is the
volumetric strain energy of confined concrete, cc is the ultimate strain of confined concrete.
The volumetric strain energy absorbed by FRP (Uf) could be determined as follows:
1 ( fefeff fU (16)
Where f is the volumetric ratio of FRP and calculated as shown in Eq. 17, Uf is the
volumetric strain energy of FRP, and ffe and fe are the actual rupture strength and rupture
strain of FRP on the columns, respectively.
The proposed strain model
The proposed strain model requires specimens including the actual rupture strain of FRP
reported. Test results of specimens not reporting the actual rupture strain of FRP were
excluded from the database. Thus, a new database (215 specimens) extracted from the full
database was used to develop the proposed strain model. The new database covers unconfined
concrete strength between 24 MPa and 112 MPa, and a variety of FRP types including CFRP,
GFRP, AFRP, HM CFRP, CFRP tube, and AFRP tube. The energy absorption of 215
specimens was determined using Eqs. 15 and 16, and the results are presented in Fig. 6. Next,
a regression analysis was undertaken to attain the following equation:
fcc U.U 626 (18)
Substituting Eqs. 15 and 16 into Eq. 18, results in the following equation:
where the proportion coefficient k is equal to 6.62. This expression could be used to calculate
the axial strain of CFRP confined concrete columns in circular sections. Using this calculated
strain, any model could be utilized to calculate the confined concrete strength. Lam and Teng
model (2003) was adopted to express another form of Eq. 19 as follows:
Verification of the strain model
Fig. 7 shows theoretical strain versus…